THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT


 Eugene Turner
 1 years ago
 Views:
Transcription
1 THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2 ETSI Aeronáuticos. Universidad Politécnica de Madrid. Madrid, Spain (28040) SUMMARY: A threedimensional finite element model of the joint has been developed. The model has been used to predict the stress field of the laminate in the joint area, assuming homogeneity and linear behavior of the material. The modeled geometry is a Tbolt that joins a coupon of glass fiber epoxy and a block of steel. The results obtained from the model have been verified experimentally using both electric and optical strain sensors. In the discussion of the results, a comparison between the stresses predicted for the Tbolt and those of an equivalent double lap bolted joint has been performed. KEYWORDS : Composite Joints, Stress Analysis, 3D Models. INTRODUCTION One of the most critical joints in a wind turbine is the joint between the blade root and the hub. While it has a great responsibility in the wind turbine performance and integrity, its inspection is very difficult and forces to stop the turbine. Another singularity of this connection is the huge thickness of the blade root laminate (typically > 60mm). On the other hand, there is a marked trend in the wind energy industry to build blades as large as possible. Therefore, over the years, there is an increase in the joint loads, but at the same time, the different elements need to be relatively lighter and cheaper. In this scope, many different solutions have been proposed, but only few of them have demonstrated to be able to fulfill all the requirements of the modern wind turbines and are being used at industrial scale. One of the most successful of these solutions is the socalled Tbolt connection, shown in figure 1. It consists mainly of the nut, i.e. a steel cylinder placed transversally to the blade root laminate, and a prestressed screw with one tip screwed to the nut and the other one connected to the rotor hub by means of standard washers. 1
2 Nut A Blade Root Hub A Screw View from the inside of the hub Section AA Fig. 1 Tbolt connection One of the main characteristics of this kind of joints is that, due to the high prestresses introduced in the screw, there is always compression under the nut, no matter whether the external load is introduced by tension or compression. Therefore, the dangerous loosening of the joint, due to reversed loads, is avoided. There are some important differences between Tbolt joints and classical overlapped joints, among others: The laminates are extremely thick: typically mm. The stress distribution in the bearing zone is clearly nonuniform through the thickness. When loaded in tension, the pretension of the screw creates a load path different to those usually found in overlapping joints (a kind of tension + compression bypass). Usually it is not possible to include any clamping pretension in the nut. Those differences make unfeasible to use the results obtained from overlapped joints to predict the Tbolt joint strength. Despite this fact, there are only a few published works about the Tbolt connection [1]. Therefore, new efforts are required in order to characterize the Tbolt behavior and its strength. Finite element model In order to characterize the stress distribution in the Tbolt a parametric FE model has been developed. It allows an easy generation of 3D FE models, for any particular set of dimensions and material properties, by simply editing a text file containing the different physical parameters as well as the meshing densities. The model has been implemented using the program MSC MARC. 2
3 The geometry presented does not correspond to a blade root, but to the test specimen shown in figure 2. This specimen has been used to verify the numerical results and will be used to investigate the failure modes of this kind of joints. The specimen consists of a laminate 37 mm thick, joined to two steel blocks by means of two equal Tbolts. Steel block Steel block Screw Nut Laminate Fig. 2 Test coupon The laminate in the vicinity of the joint has been modeled as an homogeneous orthotropic material with elastic properties equivalent to those of the laminate. Although using this assumption interlaminar stresses are neglected, it is not possible to use a one or more element per layer approach, due to the enormous number of layers involved: about 280 for a laminate 60 mm thick. Due to symmetry considerations, only 1/8 of the laminate part of the coupon has been modeled. The model uses eight node hexahedral elements with bilinear shape functions (element 21 from the MARC element library). This element class was chosen instead of more accurate quadratic elements, because of the problems arising from the use of them in contact simulations. The presence of the screw hole makes not possible to mesh the Tbolt geometry using simple radial structured meshes similar to those used for double lap bolted joints (figure 3a). Thus, automatic unstructured mesh generators were tested, but it was not possible to have a precise control over the mesh quality in the different areas of the model. Fig. 3 a) Radial structured mesh. b) Tbolt. 3
4 Therefore, an automatic structured meshing procedure for the Tbolt geometry has been developed. The mesh density in the different areas of the model is controlled by several simple variables that allow to obtain meshes with high element densities only where high stress gradients are expected (figure 3b). Using this procedure, it is possible to obtain accurate results with less than 1/5 of the nodes needed in unstructured meshes. The nut has been modeled as a rigid cylindrical surface because of the small influence of considering its stiffness on the results (the stiffness ratio between steel and the considered laminate is about 210 to 18). Therefore, the contact procedure checks whether each node in the nut hole surface penetrates the cylindrical surface. Once contact is detected, the degrees of freedom are transformed to a local system, and a constraint is imposed such that: u normal = v n, where v is the velocity of the rigid surface and n is the normal to it. The friction forces between the nut and the laminate have not been considered. Due to the pretension of the screw, the increment (P b ) of the screw tension (F b ) is only a fraction of the applied external load (P). This fraction depends on the geometry of the joint and on the stiffness ratio between the screw and the part of the laminate between the nut and the steel block. Therefore, the relative displacement between the nut and the steel block should be calculated for each load case, taking into account the applied external load (P), the initial pretension of the screw (F 0 ), the screw stiffness (K b ) and the laminate stiffness (K m ). Figure 4 shows the relations between the different parameters in the so called rigging diagram. P: external load F P f : external load at joint opening F 0: initial pretension load F b: screw tension (bearing load) F m : contact force P b P m P F b = P + F m F b = F 0 + P b K b P f F 0 F b K m F m L Fig. 4 Rigging diagram VERIFICATION In order to verify the F.E. model, a single specimen has been tested both numerically and experimentally. The geometry of the test specimen is shown in figure 2 and its dimensions are shown in the following table. D (mm) d (mm) w (mm) t (mm) L (mm) e (mm) tf (mm) Sp (avg.) Regarding to the material, the specimen was made of a glass fiber  epoxy laminate (0,+45,45,90) 42, with a fiber volume fraction V f =35%. The elastic properties of the laminate have been estimated assuming that all layers in a small laminate region are under the same in plane strains (ε xx, ε yy and ε xy ) and also the same out of plane stresses (σ zz, σ yz and σ zx ). The 4
5 resulting values are shown in the next table: E x E y E z ν xy ν yz ν zx G yz G zx (MPa) (MPa) (MPa) () () () (MPa) (MPa) (MPa) G xy The strains have been checked both at the laminate surface, at a point placed 10 mm under the bearing area of the nut (points G1 and G2 in figure 5) and inside the screw hole at a distance of 18 mm from the nut (point Op1). The points on the laminate surface have been checked using electrical strain gauges, whereas, at point Op1, an optical strain sensor based on Bragg gratings has been used. A description of the optical measurement technology can be found in [2]. G1 Op1 G2 Fig. 5 Measurement points Figure 6 shows the results obtained experimentally, without screw pretensioning, compared to the calculated with the F.E. model. As the F.E. model is symmetric, points G1 and G2 have the same numerical strain, that has been compared with the mean of the measures of both gauges. There is an error of about 15% between experimental and calculated values. This error may be due to some delaminations found in the edge of the nut hole, developed during manufacturing. These delaminations may lead to a relaxation in the stresses under the nut. Moreover, the estimated elastic properties of the laminate have not been verified experimentally. Despite this error level, a good correlation can be observed between the results obtained in the different points. P (kn) Op1 Mean G1,G2 100 Calc (ext) Calc (int) Strain x 10^6 () Fig. 6 Experiment FEM comparison 5
6 SIMPLE STRESS ANALYSIS In the following paragraphs, some results are presented and discussed for a Tbolt geometry identical to the used for verification, except on the width (w), that has been taken as 50 mm. This set of values leads to the geometry ratios (w/d, d/d, e/d ) typical of current blade root designs. For double lap bolted joints, when there is no clearance between the bolt and the laminate, the stress distribution is not dependent on the applied load [3]. But, according to figure 4, due to the pretension of the screw (F 0 ), the bearing load (F b ) will not equal the external load (P) until the opening of the joint (P P f ). In fact, for a given initial pretension (F 0 ), the ratio F b /P will continuously vary from to 1, as P increases from 0 to P f. Thus, although the stress distribution might not be dependent on the applied load (P), it will always depend on the F b /P ratio. This fact is illustrated in figure 7, where the x component of strain in the middle sections (through planes xy and zx) of the laminate are presented for a case with initial pretension F 0 =35 kn. The external load (P) is 19 kn in figure 7a, and 65kN in figure 7b, corresponding the first one to an F b /P ratio of 2, and the second one to a wide open joint (F b /P=1). While in the first case, the maximum compressive strain almost doubles the tensile one, in the second, maximum compressive and tensile strains are almost balanced. Fig. 7 a) Strains, x comp., F 0 =35 kn, P=19 kn b) Strains, x comp., F 0 =35 kn, P=65 kn Therefore, it was necessary to define which F b /P ratios should be studied. Obviously, the most interesting ratios will be those at which failure is more likely to occur. Thus, for a static analysis, the load at which opening of the joint occurs (F b /P=1) has been chosen, due to the following facts: 1. In the current Tbolt design the screw acts as a fuse, because it is the element of the joint easiest to replace. 2. If the former design criterion is used, and the fracture of the screw occurs before the opening of the joint, the maximum external load supported would be less than the maximum allowed by the screw. 3. Another important design criterion states that, in the case of laminate failure, it is always preferable a bearing failure to a net tension failure, because of the catastrophic nature of the latter. The situation where the net tension failure is more likely to appear is 6
7 at joint opening. Therefore, if the joint is designed in order to force bearing failure at joint opening, net tension fracture would not occur in any other situation. Despite its more sophisticated geometry, it is not difficult to compare the T.bolt joint to a typical double lap joint. Therefore, our first analysis consists in a comparison between the strain and stress fields of both joints in a similar load situation, with the aim of take advantage of the knowledge already available on double lap joints [4]. Figures 8 to 13 show the results for a load of 65 kn without any pretension. Both models (Tbolt and double lap) have the same geometry, except, of course, for the presence of the screw hole in the case of the Tbolt. The comparison of in plane behaviors is based on strains (ε xx, ε yy and ε xy ), while the out of plane comparison it is based on stresses (σ zz, σ yz and σ zx ). If the basic set of four layers (0,45,45,90) is thin enough, we can assume that the laminate behaves like an homogeneous orthotropic material. Therefore, the inplane strains will be the same for all layers, while the stresses will vary from one to another. Conversely, the out of plane common values will be the stresses. Fig. 8 a) Strain, x direction, Tbolt. b) Strain, x direction, double lap joint Fig. 9 a) Strain, y direction, Tbolt. b) Strain, y direction, double lap joint 7
8 Fig. 10 a) Stress, z direction, Tbolt. b) Stress, z direction, double lap joint Fig. 11 a) Shear strain, xy direction, Tbolt. b) Shear strain, xy direction, double lap joint Fig. 12 a) Shear strain, yz direction, Tbolt. b) Shear strain, yz direction, double lap joint 8
9 Fig. 13 a) Shear strain, zx direction, Tbolt. b) Shear strain, zx direction, double lap joint For all of the stress and strain components there is a high stress concentration at the intersection between the screw hole and the nut hole. These very local extreme stresses have no influence on the joint strength. Therefore, in the following discussion, we will always discard the results in this area. In general, the main stress and strain concentration areas (apart from the above mentioned) are the same for both joints. Therefore, three main stress zones should be analyzed: the net tension zone (figure 8), the bearing zone (figures 8 and 9) and the shear out zone (figure 11). Comparing both models, the following conclusions can be extracted: In the net tension zone, stresses and strains are approximately the same in both designs (figures 8 and 9). The compressive maximum strain in the Tbolt is about 1.75 times the maximum for double lap joints (figure 8). Part of this increment can be explained by the bearing area reduction caused by the screw hole (A Tbolt =A overl. /1.35). In the bearing zone, the tensile stress (y direction) is almost 2 times higher in the Tbolt (figure 9). This strain, although is not directly responsible for the bearing failure, reduces the laminate strength, producing matrix cracks and fiber failure in the 90º layer. The shearout zone is affected in two ways by the geometry of the Tbolt: first, there is a small increase in the maximum xy shear strain and, second, there is a shifting in the position where the maximum shear strain is observed (figure 11). In the Tbolt the maximum shear strain is shifted towards the bearing area. The ratio between maximum shear strains is about 1.4, and corresponds mainly to the reduction of the shear section due to the screw hole (about a factor of 1.5). There is no significative increasing in the maximum values of the stresses in the z direction compared to double lap joints (figure 10). yz and zx shear stresses appear in the neighborhood of the screw hole (figures 12 and 13). 9
10 CONCLUSIONS A three dimensional FE model has been developed for the prediction of the stresses and strains at a Tbolt joint. The model has been parameterized in order to allow an easy modification of the different geometric and elastic parameters. A simple experimental verification of the model has been conducted. Although the absolute values in the bearing zone do not completely agree with the calculated ones (15% of error), good correlation was found for the variations between different measurement points. Although for each ratio F b /P there is a different stress distribution over the laminate, only the case with F b /P = 1 has been analyzed, because it is the most critical for the strength of the joint. Comparing the Tbolt stress distribution with that of a double lap bolted joint, it is found that the net tension stresses are quite similar in both designs, while the stresses in the bearing zone are between 1.75 and 2 times higher in the Tbolt. Those increasing factors can not be explained entirely by the bearing surface reduction caused by the screw hole. Due to the higher bearing stresses, a lower joint efficiency is to be expected. On the other hand, the highest possible efficiency would appear at the transition between net tension and bearing failure, and this will occur at a much lower w/d ratio than in the case of double lap joints. Finally, some out of plane shear stresses have been found in the Tbolt model that are not present in double lap joints. These stresses may contribute to the initiation of a delamination process, but it is not possible, with the current model, to determine the relevance of these stresses compared to the interlaminar stresses in the same area. ACKNOWLEDGEMENTS This work has been supported by the Spanish government through DGICYT under the contract: MAT C We would like to thank AERPAC B.V. and AERTUSA, which have kindly provided us with fundamental data about Tbolt technology, as well as the laminate used in the experimental test. REFERENCES 1. Kensche, C. W. and Schultes, K., Evaluation of Tbolt Root Attachment, Design of Composite Structures Against Fatigue. Applications to Wind Turbine Blades, Mayer, R. M. (ed.), Mechanical Engineering Publications Limited (1996): S. DiazCarrillo, J Sancho, E. Torres, A. Guemes, Modelling and experimental analysis of thick CFRP bolted joints, ICCM13 3. Naik, R. A. and Crews, J. H., PlyLevel Failure Analysis of a Graphite/Epoxy Laminate under BearingBypass Loading, NASA TM , 135, National Aeronautics and Space Administration, Camanho, P. P. and Matthews, F. L., Stress Analysis and Strength Prediction of Mechanically Fastened Joints in FRP: a Review, Composites Part A, 28 A, ,
Openhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More informationDamage Detection in Bolted Joints by Fibre Optics Distributed Sensing
2nd International Symposium on NDT in Aerospace 2010  Mo.2.A.2 Damage Detection in Bolted Joints by Fibre Optics Distributed Sensing Alfredo GÜEMES 1*, Antonio FERNANDEZLOPEZ *1 Univ. Politecnica de
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More information2 Experiment of GFRP bolt
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FATIGUE LIFE EVALUATION OF BOLT MADE OF WOVEN FABRIC FRP Takeshi INOUE*, Hiroaki NAKAI**, Tetsusei KURASHIKI**, Masaru ZAKO**, Yuji KOMETANI*** *Graduate
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationCOMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD
10th International DAAAM Baltic Conference "INDUSTRIAL ENGINEERING  1213 May 2015, Tallinn, Estonia COMPARISON OF NUMERICAL SIMULATION AND EXPERIMENT OF A FLEXIBLE COMPOSITE CONNECTING ROD Sedláček,
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationNUMERICAL MODELING OF GAS LEAKAGE THROUGH DAMAGED COMPOSITE LAMINATES
NUMERICAL MODELING OF GAS LEAKAGE THROUGH DAMAGED COMPOSITE LAMINATES Hisashi Kumazawa*, John Whitcomb** [Hisashi Kumazawa]:kumazawa.hisashi@jaxa.jp *Structure Technology Center, Japan Aerospace Exploration
More informationFinite Element Method in Geotechnical Engineering
Finite Element Method in Geotechnical Engineering Short Course on + Dynamics Boulder, Colorado January 58, 2004 Stein Sture Professor of Civil Engineering University of Colorado at Boulder Contents Steps
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationEffects of Resin and Fabric Structure
Fatigue of Wind Blade Laminates: Effects of Resin and Fabric Structure Details David Miller, Daniel D. Samborsky and John F. Mandell Montana State t University it MCARE 2012 Outline Overview of MSU Fatigue
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More informationBEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS
BEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS Euler S. Dias*, Carlos A. Cimini Jr.* * Federal University of Minas Gerais, Dept. of Structural Engineering, Belo Horizonte 
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationINITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS INITIATION AND PROPAGATION OF FIBER FAILURE IN COMPOSITE LAMINATES E. Iarve 1,2*, D. Mollenhauer 1, T. Breitzman 1, K. Hoos 2, M. Swindeman 2 1
More informationNUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET
NUMERICAL INVESTIGATION OF DELAMINATION IN LSHAPED CROSSPLY COMPOSITE BRACKET M.Gümüş a*, B.Gözlüklü a, D.Çöker a a Department of Aerospace Eng., METU, Ankara, Turkey *mert.gumus@metu.edu.tr Keywords:
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationPREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
FONDATĂ 1976 THE ANNALS OF DUNAREA DE JOS UNIVERSITY OF GALATI. FASCICLE IX. METALLURGY AND MATERIALS SCIENCE N 0. 007, ISSN 15 08X PREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
More information15 INTERLAMINAR STRESSES
15 INTERLAMINAR STRESSES 151 OUTOFPLANE STRESSES Classical laminate plate theor predicts the stresses in the plane of the lamina,, and τ but does not account for outofplane stresses, τ and τ. It assumes
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationPredicting Failure of Multiangle Composite Laminates
Predicting Failure of Multiangle Composite Laminates Preliminary discussion (not in textbook): Micromechanics failure analyses vs Macromechanics failure analyses Fiber Architecture of Some Common Composite
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationCrack Tip Plastic Zone under Mode I Loading and the Nonsingular T zz stress
Crack Tip Plastic Zone under Mode Loading and the Nonsingular T stress Yu.G. Matvienko Mechanical Engineering Research nstitute of the Russian Academy of Sciences Email: ygmatvienko@gmail.com Abstract:
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationRELIABILITY ANALYSIS IN BOLTED COMPOSITE JOINTS WITH SHIMMING MATERIAL
25 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES RELIABILITY ANALYSIS IN BOLTED COMPOSITE JOINTS WITH SHIMMING MATERIAL P. Caracciolo, G. Kuhlmann AIRBUSGermany email: paola.caracciolo@airbus.com
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationCOMBINED INPLANE AND THROUGHTHETHICKNESS ANALYSIS FOR FAILURE PREDICTION OF BOLTED COMPOSITE JOINTS
COMBINED INPLANE AND THROUGHTHETHICKNESS ANALYSIS FOR FAILURE PREDICTION OF BOLTED COMPOSITE JOINTS V. Kradinov, * E. Madenci The University of Arizona, Tucson, Arizona, 8575 D. R. Ambur NASA Langley
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationACDC. User Manual. Ver. 1.0
ACDC User Manual Ver. 1.0 Centre Composite December 2016 ACDC, Ver. 1.0 User Manual Centre Composite, 2016 (software@composite.lv) Table of Contents Introduction... 1 System requirements... 1 Theoretical
More informationAnalysis of a Lap Joint Including Fastener Hole Residual Stress Effects
Analysis of a Lap Joint Including Fastener Hole Residual Stress Effects Guillaume Renaud, Gang Li, Guoqin Shi, Yan Bombardier, Min Liao Aerospace Portfolio AFGROW User Workshop 214, Layton, UT, September
More informationNumerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure
Copyright c 007 ICCES ICCES, vol.1, no.3, pp.9398, 007 Numerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure C. Bisagni 1 Summary The research here
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationFEAnalysis of Stringertofloorbeam Connections in Riveted Railway Bridges
FEAnalysis of Stringertofloorbeam Connections in Riveted Railway Bridges By Mohammad AlEmrani 1 and Robert Kliger 2 Department of Structural Engineering Chalmers University of Technology, SE412 96
More informationProblem " Â F y = 0. ) R A + 2R B + R C = 200 kn ) 2R A + 2R B = 200 kn [using symmetry R A = R C ] ) R A + R B = 100 kn
Problem 0. Three cables are attached as shown. Determine the reactions in the supports. Assume R B as redundant. Also, L AD L CD cos 60 m m. uation of uilibrium: + " Â F y 0 ) R A cos 60 + R B + R C cos
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationThe numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure
5th International Conference on Civil, Architectural and Hydraulic Engineering (ICCAHE 2016) The numerical simulation research of an UltraLight Photovoltaic Cell multilayer composite structure Kangwen
More informationMechanical Properties of Materials
Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationDynamic Response Of Laminated Composite Shells Subjected To Impulsive Loads
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 14, Issue 3 Ver. I (May.  June. 2017), PP 108123 www.iosrjournals.org Dynamic Response Of Laminated
More informationSKINSTRINGER DEBONDING AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS
SKINSTRINER DEBONDIN AND DELAMINATION ANALYSIS IN COMPOSITE STIFFENED SHELLS R. Rikards, K. Kalnins & O. Ozolinsh Institute of Materials and Structures, Riga Technical University, Riga 1658, Latvia ABSTRACT
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationCOMELD TM JOINTS: A NOVEL TECHNIQUE FOR BONDING COMPOSITES AND METAL
COMELD TM JOINTS: A NOVEL TECHNIQUE FOR BONDING COMPOSITES AND METAL F.J. Guild *, P.J. Hogg + and W. Tu School of Engineering and Materials Science, Queen Mary, University of London, London E1 4NS, UK
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationMECHANICS OF MATERIALS
CHATR Stress MCHANICS OF MATRIALS and Strain Axial Loading Stress & Strain: Axial Loading Suitability of a structure or machine may depend on the deformations in the structure as well as the stresses induced
More informationFracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach
University of Liège Aerospace & Mechanical Engineering Fracture Mechanics, Damage and Fatigue Linear Elastic Fracture Mechanics  Energetic Approach Ludovic Noels Computational & Multiscale Mechanics of
More informationMechanical analysis of timber connection using 3D finite element model
Mechanical analysis of timber connection using 3D finite element model Bohan XU Ph.D Student Civil Engineering Laboratory (CUST) ClermontFerrand, France Mustapha TAAZOUNT DrIng Civil Engineering Laboratory
More informationDrilling in tempered glass modelling and experiments
Drilling in tempered glass modelling and experiments Jens H. NIELSEN* * Department of Civil Engineering, Technical University of Denmark jhn@byg.dtu.dk Abstract The present paper reports experimentally
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationNumerical Evaluation of Fracture in Woven Composites by Using Properties of Unidirectional Type for modelling
J. Basic. Appl. Sci. Res., 2(12)1320213209, 2012 2012, TextRoad Publication ISSN 20904304 Journal of Basic and Applied Scientific Research www.textroad.com Numerical Evaluation of Fracture in Woven Composites
More informationCHAPTER 7 FINITE ELEMENT ANALYSIS OF DEEP GROOVE BALL BEARING
113 CHAPTER 7 FINITE ELEMENT ANALYSIS OF DEEP GROOVE BALL BEARING 7. 1 INTRODUCTION Finite element computational methodology for rolling contact analysis of the bearing was proposed and it has several
More informationTENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES
TENSILE FATIGUE BEHAVIOR OF SINGLE FIBRES AND FIBRE BUNDLES C. Qian 1 *, R. P. L. Nijssen 1, D. D. Samborsky 2, C.Kassapoglou 3, Z. Gürdal 3, G. Q. Zhang 4 1 Knowledge Centre Wind turbine Materials and
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationStrength of GRPlaminates with multiple fragment damages
Strength of GRPlaminates with multiple fragment damages S. Kazemahvazi, J. Kiele, D. Zenkert Kungliga Tekniska Högskolan, KTH 100 44 Stockholm, Sweden sohrabk@kth.se SUMMARY The strength of glass fibre
More informationEXPERIMENTAL AND THEORETICAL STUDY OF THE DAMAGE ONSET IN BIAXIAL CRUCIFORM SPECIMENS UNDER STATIC AND HYSTERESIS LOADING
EXPERIMENTAL AND THEORETICAL STUDY OF THE DAMAGE ONSET IN BIAXIAL CRUCIFORM SPECIMENS UNDER STATIC AND HYSTERESIS LOADING E. Lamkanfi a,1, C. Ramault 2, A. Makris 2, W. Van Paepegem 1, J. Degrieck 1, D.
More informationKeywords: Adhesively bonded joint, laminates, CFRP, stacking sequence
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS GLOBAL AND LOCAL INFLUENCE OF STACKING SEQUENCE ON THE STRENGTH OF ADHESIVELY BONDED JOINTS OF CFRP LAMINATES J. Rousseau*, P. Satthamnuwong DRIVE,
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationAERSYS KNOWLEDGE UNIT
7016 1. INTRODUCTION The scope of this document is to provide a clarification and a deeper understanding of the two different ways to move the mid plane of the element out of the nodal plane. Although
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationA fatigue design methodology for GRP composites in offshore underwater applications
A fatigue design methodology for GRP composites in offshore underwater applications Dr P. A. FRIEZE P A F A Consulting Engineers Limited, Hampton, Middx, UK INTRODUCTION Norsk Hydro Troll C field  floating
More informationNUMERICAL SIMULATION OF FLANGEBOLT INTERACTION IN WIND TUBRINE TOWER CONNECTIONS
8 th International Congress on Computational Mechanics Volos, 12 July 15 July 2015 NUMERICAL SIMULATION OF FLANGEBOLT INTERACTION IN WIND TUBRINE TOWER CONNECTIONS Aikaterini I. Ntaifoti 1, Konstantina
More informationINTERFACIAL STRENGTH EVALUATION IN A GLASS FIBER REINFORCED COMPOSITE USING CRUCIFORM SPECIMEN METHOD
INTERFACIAL STRENGTH EVALUATION IN A GLASS FIBER REINFORCED COMPOSITE USING CRUCIFORM SPECIMEN METHOD Shinji Ogihara, oriaki Sakamoto 2, Hajime Kato 2, Satoshi Kobayashi 3 and Ichiro Ueno Dept. of Mechanical
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each.
GTE 2016 Q. 1 Q. 9 carry one mark each. D : SOLID MECHNICS Q.1 single degree of freedom vibrating system has mass of 5 kg, stiffness of 500 N/m and damping coefficient of 100 Ns/m. To make the system
More informationExperimental Study and Numerical Simulation on Steel Plate Girders With Deep Section
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 12, 2015, University of
More informationEFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES
EFFECT OF ELLIPTIC OR CIRCULAR HOLES ON THE STRESS DISTRIBUTION IN PLATES OF WOOD OR PLYWOOD CONSIDERED AS ORTHOTROPIC MATERIALS Information Revied and Reaffirmed March 1956 No. 1510 EFFECT OF ELLIPTIC
More informationFinite Element Analyses of Low Velocity Impact on Thin Composite Disks
International Journal of Composite Materials 2013, 3(6B): 5970 DOI: 10.5923/s.cmaterials.201310.07 Finite Element Analyses of Low Velocity Impact on Thin Composite Disks Marcelo L. Ribeiro 1, Ricardo
More informationDynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load
Dynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,
More informationStructural behaviour of traditional mortiseandtenon timber joints
Structural behaviour of traditional mortiseandtenon timber joints Artur O. Feio 1, Paulo B. Lourenço 2 and José S. Machado 3 1 CCR Construtora S.A., Portugal University Lusíada, Portugal 2 University
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More information